data_1000066
_cod_database_code               1010298
_structure_refined               no
_mpod_phase_name                 ?
_mpod_phase_generic_name         Nd:SGGM
_chemical_formula_sum            'Nd0.0136 Sr0.92 Gd1.01 Ga2.88 O7'
_mpod_symmetry_point_group_name_h-m '-4 2 m'
_cell_length_a                   7.972
_cell_length_c                   5.251
loop_
_publ_author_name
'Zhang, Y.Y.'
'Zhang, H.J.'
'Yu, H.H.'
'Wang, J.Y.'
'Gao, W.L.'
'Xu, M.'
'Sun, S.Q.'
'Jiang, M.H.'
'Boughton, R.I.'
_publ_section_title
;
 Synthesis, growth, and characterization of Nd-doped SrGdGa3O7 crystal
;
_journal_name_full               'Journal of Applied Physics'
_journal_volume                  108
_journal_issue                   6
_journal_article_reference       063534
_journal_pages_number            10
_journal_year                    2010
_mpod_phase_density              5634
data_1000066a
loop_
_prop_conditions_label
_prop_conditions_temperature
1 303.1
2 560.6
3 304
4 560.2
5 303
loop_
_prop_thermal_tensorial_index
_prop_thermal_condition_label
_prop_thermal_measurement_method
_prop_thermal_conductivity_kappaij
_prop_thermal_diffusivity_kappadij
11 5 LPM ? 0.00000067
22 5 LPM ? 0.00000067
33 5 LPM ? 0.00000059
11 1 LPM 1.59 ?
22 1 LPM 1.59 ?
33 1 LPM ? ?
11 3 LPM ? ?
22 3 LPM ? ?
33 3 LPM 1.40 ?
11 4 LPM ? ?
22 4 LPM ? ?
33 4 LPM 1.96 ?
11 2 LPM 2.12 ?
22 2 LPM 2.12 ?
33 2 LPM ? ?
data_1000066b
loop_
_prop_conditions_label
_prop_conditions_temperature_range_begin
_prop_conditions_temperature_range_end
1 303 773
loop_
_prop_thermal_tensorial_index
_prop_thermal_condition_label
_prop_thermal_measurement_method
_prop_thermal_expansion_alphaij
11 1 SCXD 5.32
22 1 SCXD 5.32
33 1 SCXD 5.65
data_1000066c
loop_
_prop_conditions_label
_prop_conditions_temperature
1 303
loop_
_prop_heat_capacity_tensorial_index
_prop_heat_capacity_condition_label
_prop_heat_capacity_measurement_method
_prop_heat_capacity_C
. 1 DSC 0.419
data_1000066d
loop_
_prop_conditions_label
_prop_conditions_wavelength
1 0.2537
10 0.8521
11 1.014
12 1.530
13 2.325
2 0.363
3 0.4047
4 0.4358
5 0.480
6 0.5461
7 0.5875
8 0.6438
9 0.7065
loop_
_prop_optical_tensorial_index
_prop_optical_condition_label
_prop_optical_measurement_method
_prop_optical_index_extraordinary_ne
_prop_optical_index_ordinary_no
. 1 MDT 2.0616061 2.0379258
. 2 MDT 1.9066923 1.9012401
. 3 MDT 1.8864119 1.8793089
. 4 MDT 1.8749420 1.8670582
. 5 MDT 1.8629145 1.8543279
. 6 MDT 1.8506377 1.8414330
. 7 MDT 1.8451414 1.8357980
. 8 MDT 1.8393703 1.8296930
. 9 MDT 1.8345550 1.8246548
. 10 MDT 1.8272175 1.8170938
. 11 MDT 1.8222021 1.8118757
. 12 MDT 1.8139621 1.8033156
. 13 MDT 1.8057108 1.7946656
